© 2012 Chan et al., licensee InTech. This is an open access chapter distributed under the terms of the
Creative Commons Attribution License (http://creativecommons.org/licenses/by/3.0), which permits
unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Poly(trimethylene terephthalate) –
The New Generation of Engineering
Chin Han Chan, Sarathchandran and Sabu Thomas
Additional information is available at the end of the chapter
Polyester is the category of polymers with ester functional group on the main chain,
although there are many types of polyester, the term polyester in industries specifically
refers to poly(ethylene terephthalate) (PET) and poly(butylene terephthalate). Polyesters can
be classified as thermoplastic or thermosetting depending on the chemical structures. Table
1 shows the industrial production of polyesters, and it is estimated that the production will
exceed 50 million tons by the year of 2015. Polyesters are made from chemical substances
found mainly in petroleum and are mainly manufactured into fibers, films, and plastics.
These polyesters are abbreviated as mGT, where m denotes the number of methylene
groups; e.g.: PET, Poly(trimethylene terephthalate) (PTT) and PBT are abbreviated as 2GT,
3GT and 4GT, respectively.
Market size per year
Product type 2002 [Million tons/year] 2008 [Million tons/year]
Textile-PET 20 39
(solution casted PET)
Film-PET 1.2 1.5
Special polyester 1 2.5
Total 31.2 49
Table 1. The world production of polyester
The credit of finding that alcohols and carboxylic acids can be mixed successfully to create
fibers goes to W.H.Carothers, who was working for DuPont at the time and unfortunately
when he discovered Nylon, polyester took a back seat. Carothers’s incomplete research had
not advanced to investigating the polyester formed from mixing ethylene glycol and
terephthalic acid. It was the two British scientists – Whinfield and Dickson who patented
PET in 1941. Later that year, the first polyester fiber – Terylene – was synthesized by
Whinfield and Dickson along with Birtwhistle and Ritchiethey. Terylene was first
manufactured by Imperial Chemical Industries or ICI. PET forms the basis of synthetic
fibers like Dacron, Terylene and polyesters. DuPont's polyester research lead to a whole
range of trademarked products, one example is Mylar (1952), an extraordinarily strong PET
fiber that grew out of the development of Dacron in the early 1950s.
The industrial production of polyesters involves three steps
1. Condensation Polymerization: When acid and alcohol are reacted in vacuum, at high
temperatures condensation polymerization takes place. After the polymerization, the
material is extruded onto a casting trough in the form of ribbon. Upon cooling, the
ribbon hardens and is cut into chips.
2. Melt-spun Fiber: The chips are dried completely. Hopper reservoirs are then used to
melt the chips. Afterwards, the molten polymer is extruded through spinnerets and
cooled down by air blowing. It is then loosely wound around cylinders.
3. Drawing: The fibers consequently formed are hot stretched to about five times of their
original length (to reduce the fiber width). This is then converted into products.
PTT is an aromatic polyester prepared by the melt polycondensation of 1, 3-propanediol
(PDO) with either terephthalic acid (TPA) or dimethyl terephthalate (DMT). PTT is
synthesized by the transesterification of propane diol with dimethylene terephthalate or by
the esterification of propane diol with terephthalic acid. The reaction is carried out in the
presence of hot catalyst like titanium butoxide and dibutyl tin oxide at a temperature of 260
oC. The important by-products of this reaction include acrolien and allyl alcohol. Direct
esterification of propane diol and terephthalic acid is considered as the least economic and
industrial method. The reaction is carried out in the presence of a “heel” under a pressure of
70-150 kPa at a temperature of 260 oC. The “heel” is usually referred to the added PTT
oligomers which act as a reaction medium and increase the solubility of terephthalic acid.
Recent studies by different groups show that the selection of the catalyst plays a major role
on the reaction rate and PTT properties. Commonly used catalysts like titanium, tin[5, 6] and
antimony[7, 8] compounds have their own limitations. Titanium-based catalysts are active but
the PTT is discolored, antimony-based catalysts are toxic and only active in
polycondensation while tin-based compounds have lower catalytic activity. G. P.
Karayannidis and co-workers (2003) reported the use of stannous octoate as the catalyst for
PTT synthesis but its catalytic activity is poor, resulting in a low molecular weight PTT
which was confirmed by measuring the content of terminal carboxyl groups. In this study,
the catalytic activity was followed by measuring the amount of water generated and
characterized by the degree of esterification (DE). Intrinsic viscosity measurement was
carried out by using an Ubbelohde viscometer at 25 oC with 0.005 g mL-1 PTT solution of 1,
1, 2, 2-tetrachloroethane/phenol (50/50, w/w) mixture. The content of terminal carboxyl
Poly(trimethylene terephthalate) – The New Generation of Engineering Thermoplastic Polyester 21
group (CTCG) was determined by titrating 25 mL of chloroform and a few drops of
phenolphthalein indicator to a solution of 1.000 g of PTT and 25 mL of benzyl alcohol
against a titer of 0.561 g of KOH in 1 L of benzyl alcohol.
([η]) (dL g-1)
CTCG (mol t-1)
after 1.8 hr
Stannous oxalate (SnC2O4) 0.8950 15 97
0.6155 34 75
Dibutyltin oxide (Bu2SnO) 0.8192 21 75
Tetrabutyl titanate 0.8491 20 82
Table 2. Effect of various catalysts on the properties of PTT. The amount of catalyst taken was 5·10-4
mol/mol of TPA, and esterification for 1.6 hrs; at 230 oC .
Works by different groups show that stannous oxalate is one of the best for PET and
PBT syntheses and also a potential additive for improving the properties of the
polymers. Studies by J. S. Yong et al. (2008) who used stannous oxalate as the catalyst to
synthesize PTT. The results show that stannous oxalate (SnC2O4) displays higher
polymerization activity than the other catalysts which is clear by the fact that SnC2O4 shows
the highest intrinsic viscosity ([η]) and lowest content of terminal carboxyl groups (ref. Table
2). Decrease in reaction time and improvement in PTT property are observed as shown in
Table 2 and Fig. 2. The higher catalytic activity of SnC2O4 is attributed to its chelate
molecular structure and suggests SnC2O4 as a more promising catalyst for PTT synthesis.
The chemical structures of different catalysts used are shown in Fig. 1.
Figure 1. Chemical structure of the catalysts used for PTT synthesis.
0.0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8
Figure 2. Effect of different catalysts on esterification TPA. The amount of catalyst used was 5·10-4
mol/mol of TPA. Parameter DE denotes degree of esterification.
In the industrial synthesis, the process of melt polycondensation has the disadvantages of
high melt viscosity and difficulty in removal of the by-products which often limits the
desirable molecular weight of the polymer. Specially designed reactor (e.g., disk-ring
reactor) is required for the melt polycondensation process in most cases in providing large
liquid surface area along with the application of high vacuum for rapid removal of by-
products. J. K. Yong et al. (2012) proposed the use of solid-state polymerization as a
potential technique to overcome the limitations of the melt polycondensation process. For
the synthesis of PTT, low molecular weight polymer (pre polymer) is first synthesized by
melt esterification or melt transesterification at low temperatures. The pre polymer is then
ground or pelletized and is crystallized to prevent particle agglomeration during solid state
polymerization, with subsequent heating to a temperature above the glass transition
temperature (Tg) and below the melting temperature (Tm) of the pre polymer. This is
explained on the basis of negligible diffusion resistance offered by the use of sufficiently
small sized particles. Highest rate is observed when the pre polymer is used, which has zero
carboxylic acid content.
Although PTT is reported in the early 1950s, interest in commercialization of PTT began
with the introduction of relatively new methods for the synthesis of propane diol by the
catalytic hydrogenation of intermediate 3-hydroxypropionaldehyde and hydroformylation
of ethylene oxide. Recent discovery of fermentive production of 1, 3-propane diol
accelerates the interest of studying PTT for engineering applications[15, 16].
PTT is a rapidly crystallizing linear aromatic polyester. Differential scanning calorimeter
(DSC) studies by P. D. Hong et al. (2002) using completely amorphous PTT ( nM = 43, 000
Poly(trimethylene terephthalate) – The New Generation of Engin